1 / 48

490 likes | 717 Views

Density, Volume, and Packing: Part 2 Thursday, September 4, 2008. Steve Feller Coe College Physics Department. Lecture 3 of Glass Properties Course. Some Definitions. x = molar fraction of alkali or alkaline-earth oxide (or any modifying oxide) 1-x = molar fraction of glass former

Download Presentation
## Density, Volume, and Packing: Part 2 Thursday, September 4, 2008

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**Density, Volume, and Packing: Part 2Thursday, September 4,**2008 Steve Feller Coe College Physics Department Lecture 3 of Glass Properties Course**Some Definitions**• x = molar fraction of alkali or alkaline-earth oxide (or any modifying oxide) • 1-x = molar fraction of glass former • R = x/(1-x) This is the compositional parameter of choice in developing structural models for borates. • J = x/(1-x) for silicates and germanates**Short Ranges B and Si Structures**Short-range borate units, Short-range silicate units,**Method of Least Squares**• Take (ρmod – ρexp)2 for each data point • Add up all terms • Vary volumes until a least sum is found. • Volumes include empty space. • ρmod = M/(fiVi)**Example: Li-Silicates**VQ4 = 1.00 VQ3 = 1.17 VQ2 = 1.41 VQ1 = 1.69 VQ0 = 1.95 VQ4(J = 0) defined to be 1. The J = 0 glass is silicon dioxide with density of 2.205 g/cc**Borate Structural Model**• R < 0.5 • F1 = 1-R, F2 = R • 0.5 <R <1.0 • F1 = 1-R, F2 = -(1/3)R +2/3, F3 = +(4/3)R -2/3 • 1.0 <R < 2.0 • F2 = -(1/3)R +2/3, F3 = -(2/3)R +4/3 , F4 = R-1**Another Example: Li-Borates**• V1 = 0.98 • V2 = 0.91 • V3 = 1.37 • V4 = 1.66 • V5 = 1.95 • V1(R = 0) is defined to be 1. • The R = 0 glass is boron oxide with density of 1.823 g/cc**Li and Ca Silicates**Li Ca VQ4 = 1.00 VQ4 = 1.00 VQ3 = 1.17 VQ3 = 1.20 VQ2 = 1.41 VQ2 = 1.46 VQ4(J = 0) defined to be 1. The J = 0 glass is silicon dioxide with density of 2.205 g/cc**Densities of Barium Borate Glasses**• R = x/(1-x) Density (g/cc) • 0·0 1·82 • 0·2 2·68 • 0·2 2·66 • 0·4 3·35 • 0·4 3·29 • 0·6 3·71 • 0·6 3·68 • 0·8 3·95 • 0·8 3·90 • 0·9 4·09 • 1·2 4·22 • 1·3 4·31 • 1·5 4·40 • 1·7 4·50 • 2·0 4·53 Use these data and the borate model to find the four borate volumes. Note this model might not yield exactly the volumes given before.**Volumes and packing fractions of borate short-range order**groups. The volumes are reported relative to the volume of the BO1.5 unit in B2O3 glass. Packing fractions were determined from the density derived volumes and Shannon radii[i],[ii]. • System Unit Least Squares Volumes Packing Fraction • Li f1 0.98 0.34 • f2 0.94 0.65 • f3 1.28 0.39 • f4 1.61 0.41 • Na f1 0.95 0.35 • f2 1.24 0.62 • f3 1.58 0.41 • f4 2.12 0.46 • K f1 0.95 0.35 • f2 1.66 0.69 • f3 1.99 0.52 • f4 2.95 0.59 • Rb f1 0.98 0.34 • f2 1.92 0.67 • f3 2.27 0.52 • f4 3.41 0.59 • Cs f1 0.97 0.34 • f2 2.28 0.67 • f3 2.62 0.54 • f4 4.13 0.61 • [i] Barsoum, Michael, Fundamentals of Ceramics (McGraw-Hill: Columbus OH,1997), 85-89. • [ii] R.D. Shannon, Acta. Crystallogr., A32 (1976), 751.**System Unit Least Squares Volumes Packing Fraction**• Mg f1 0.98 0.34 • f2 0.95 0.63 • f3 1.26 0.39 • f4 1.46 0.44 • Ca f1 0.98 0.34 • f2 0.95 0.71 • f3 1.28 0.44 • f4 1.66 0.48 • Sr f1 0.94 0.36 • f2 1.08 0.68 • f3 1.41 0.45 • f4 1.92 0.48 • Ba f1 0.97 0.35 • f2 1.13 0.73 • f3 1.55 0.47 • f4 2.16 0.51**Volumes and packing fractions of silicates short-range**order groups. The volumes are reported relative to the volume of the Q4 unit in SiO2 glass. Packing fractions were determined from the density derived volumes and Shannon radii4,23. • System Unit Least Squares Volumes Packing Fraction • Li Q4 1.00 0.33 • Q3 1.17 0.38 • Q2 1.41 0.41 • Q1 1.67 0.42 • Q0 1.92 0.43 • Na Q4 1.00 0.33 • Q3 1.34 0.42 • Q2 1.74 0.46 • Q1 2.17 0.48 • Q0 2.63 0.49 • K Q4 0.99 0.33 • Q3 1.58 0.52 • Q2 2.27 0.58 • Q1 2.97 0.61 • Rb Q4 1.00 0.33 • Q3 1.72 0.53 • Q2 2.63 0.57 • Q1 3.53 0.59 • Cs Q4 0.98 0.33 • Q3 1.96 0.56 • Q2 2.90 0.64 • Q1 4.25 0.62**Alkali Thioborates**• Data from Prof. Steve Martin • x M2S.(1-x)B2S3 glasses • Unusual F2 behavior**Volumes and packing fractions of thioborate short-range**order groups. The volumes are reported relative to the volume of the BS1.5 unit in B2S3 glass. • System Unit Least Squares Volumes Corresponding Oxide Volume • (compared with volume of BO1.5 unit in B2O3 glass.) • __________________________ • Na f1 1.00 0.95 • f2 1.37 1.24 • f3 1.51 1.58 • f5 2.95 2.66* • K f1 1.00 0.95 • f2 1.65 1.66 • f3 1.78 1.99 • f5 3.53 3.91* • Rb f1 1.00 0.98 • f2 1.79 1.92 • f3 1.97 2.27 • f5 3.90 4.55* • Cs f1 1.00 0.97 • f2 1.83 2.28 • f3 2.14 2.62 • f5 4.46 5.64* • *extrapolated**Molar Volume**• Molar Volume = Molar Mass/density It is the volume per mole glass. It eliminates mass from the density and uses equal number of particles for comparison purposes.**Borate Glasses**Kodama Data**Problem:**• Calculate the molar volumes of the barium borates given before. You will need atomic masses. Also, remember that the data are given in terms of R and there are R+1 moles of glassy materials. You could also use x to do the calculation.**Li-Vanadate (yellow) Molar Volumes campared with**Li-Phosphates (black)**Rb -purple squares**Cs -yellow triangles**K- open circles**Rb -purple squares Cs -yellow triangles**Differential Changes in Unit Volumes**• To begin the calculation, we define the glass density in terms of its dimensionless mass relative to pure borate glass (R=0), m′(R), and its dimensionless volume relative to pure borate glass, v′(R):**Solve for v1 and v2 simultaneously and assign it to R = (R1**+R2)/2 • This is accurate if R1 and R2 are close to each other; in Kodama’s data this condition is met.**The Volume per Mole Glass Former**• Volume per mole glass former = Mass (JM2O.SiO2)/density It is the volume per mole glass former and R moles of modifier.**The Volume per Mole Glass Former**• Why is there a trend linear? • JM2O.SiO2 (1-2J)Q4 +2JQ3J<0.5 • So slope of volume curve is the additional volume needed to form Q3 at the expense of Q4. This is proportional to J.**Sodium Borogermanates Volumes per Mol B2O3 Compared to**Sodium Borosilicates**Problem**• For the barium borate data provided earlier plot the volume per mol boron oxide as a function of R. • How do you interpret the result? Lecture 2 ends here**Packing in Glass**• We will now examine the packing fractions obtained in glasses. This will provide a dimensionless parameter that displays some universal trends. • We will need a good knowledge of the ionic radii. This will be provided next.

More Related